#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/12/4301240.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4301240
loop_
_publ_author_name
'Hans-Conrad zur Loye'
'Tara J. Hansen'
'Qingbiao Zhao'
'Samuel J. Mugavero'
'Ray L. Withers'
'Mark D. Smith'
_publ_section_title
;
Crystal Growth of Novel Lanthanide-Containing Platinates K4[Ln6Pt2O15] (Ln
= La, Pr, Nd, Sm) with a Unique Framework Structure
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              414
_journal_page_last               416
_journal_paper_doi               10.1021/ic801789e
_journal_volume                  48
_journal_year                    2009
_chemical_formula_moiety         '(K4.18, O0.50), La6 O15 Pt2'
_chemical_formula_sum            'K4.18 La6 O15.5 Pt2'
_chemical_formula_weight         1634.88
_chemical_name_systematic
; 



 ? 



;
_space_group_IT_number           229
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.1552(1)
_cell_length_b                   12.1552(1)
_cell_length_c                   12.1552(1)
_cell_measurement_reflns_used    6338
_cell_measurement_temperature    294(2)
_cell_measurement_theta_max      39.432
_cell_measurement_theta_min      2.369
_cell_volume                     1795.92(3)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.625 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  'SHELXTL Version 6.14 (Bruker, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      294(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0539
_diffrn_reflns_av_sigmaI/netI    0.0151
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            22480
_diffrn_reflns_theta_full        40.23
_diffrn_reflns_theta_max         40.23
_diffrn_reflns_theta_min         2.37
_exptl_absorpt_coefficient_mu    30.489
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4916
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    6.047
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cube
_exptl_crystal_F_000             2805
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.384
_refine_diff_density_min         -1.435
_refine_diff_density_rms         0.280
_refine_ls_extinction_coef       0.00021(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.129
_refine_ls_matrix_type           full
_refine_ls_number_parameters     29
_refine_ls_number_reflns         598
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.129
_refine_ls_R_factor_all          0.0251
_refine_ls_R_factor_gt           0.0218
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0180P)²+28.4252P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0463
_refine_ls_wR_factor_ref         0.0479
_reflns_number_gt                554
_reflns_number_total             598
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801789e_si_001_4.cif
_cod_data_source_block           th4139as
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_formula_sum        'K4.18 La6 O15.50 Pt2'
_cod_database_code               4301240
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-x+1/2, -z+1/2, y+1/2'
'x+1/2, -z+1/2, -y+1/2'
'x+1/2, z+1/2, y+1/2'
'-x+1/2, z+1/2, -y+1/2'
'-z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, -x+1/2'
'z+1/2, y+1/2, x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0.2500 0.2500 0.2500 0.00621(7) Uani 1 12 d S . .
La1 La 0.0000 0.297163(19) 0.297163(19) 0.00872(8) Uani 1 4 d S . .
O1 O 0.13911(17) 0.13911(17) 0.3100(3) 0.0105(5) Uani 1 2 d S . .
O2 O 0.2500 0.0000 0.5000 0.0134(11) Uani 1 8 d S . .
O3 O 0.0000 0.0000 0.0000 0.028(4) Uani 1 48 d S . .
K1 K 0.2155(3) 0.0000 0.0000 0.0231(7) Uani 0.845(11) 8 d SP . .
K2 K 0.373(2) 0.0000 0.0000 0.025(6) Uani 0.149(15) 8 d SP . .
K3 K 0.4659(11) 0.0000 0.0000 0.047(5) Uani 0.396(14) 8 d SP . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pt Pt -1.7033 8.3905 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Pt1 O1 87.95(12) . 81 ?
O1 Pt1 O1 92.05(12) . 9 ?
O1 Pt1 O1 180.0 81 9 ?
O1 Pt1 O1 87.95(12) . 77 ?
O1 Pt1 O1 92.06(12) 81 77 ?
O1 Pt1 O1 87.94(12) 9 77 ?
O1 Pt1 O1 92.05(12) . 5 ?
O1 Pt1 O1 87.94(12) 81 5 ?
O1 Pt1 O1 92.06(12) 9 5 ?
O1 Pt1 O1 180.00(9) 77 5 ?
O1 Pt1 O1 180.0 . 73 ?
O1 Pt1 O1 92.06(12) 81 73 ?
O1 Pt1 O1 87.94(12) 9 73 ?
O1 Pt1 O1 92.06(12) 77 73 ?
O1 Pt1 O1 87.94(12) 5 73 ?
O1 Pt1 La1 54.35(6) . . ?
O1 Pt1 La1 125.652(4) 81 . ?
O1 Pt1 La1 54.35(6) 9 . ?
O1 Pt1 La1 54.12(9) 77 . ?
O1 Pt1 La1 125.88(9) 5 . ?
O1 Pt1 La1 125.652(4) 73 . ?
O1 Pt1 La1 54.12(9) . 81 ?
O1 Pt1 La1 54.35(6) 81 81 ?
O1 Pt1 La1 125.651(4) 9 81 ?
O1 Pt1 La1 54.35(6) 77 81 ?
O1 Pt1 La1 125.651(4) 5 81 ?
O1 Pt1 La1 125.88(9) 73 81 ?
La1 Pt1 La1 71.397(6) . 81 ?
O1 Pt1 La1 125.88(9) . 9 ?
O1 Pt1 La1 125.651(4) 81 9 ?
O1 Pt1 La1 54.35(6) 9 9 ?
O1 Pt1 La1 125.651(4) 77 9 ?
O1 Pt1 La1 54.35(6) 5 9 ?
O1 Pt1 La1 54.12(9) 73 9 ?
La1 Pt1 La1 108.603(6) . 9 ?
La1 Pt1 La1 180.0 81 9 ?
O1 Pt1 La1 125.651(4) . 77 ?
O1 Pt1 La1 125.88(9) 81 77 ?
O1 Pt1 La1 54.12(9) 9 77 ?
O1 Pt1 La1 54.35(6) 77 77 ?
O1 Pt1 La1 125.651(4) 5 77 ?
O1 Pt1 La1 54.35(6) 73 77 ?
La1 Pt1 La1 71.397(6) . 77 ?
La1 Pt1 La1 108.604(6) 81 77 ?
La1 Pt1 La1 71.396(6) 9 77 ?
O1 Pt1 La1 54.35(6) . 5 ?
O1 Pt1 La1 54.12(9) 81 5 ?
O1 Pt1 La1 125.88(9) 9 5 ?
O1 Pt1 La1 125.651(4) 77 5 ?
O1 Pt1 La1 54.35(6) 5 5 ?
O1 Pt1 La1 125.651(4) 73 5 ?
La1 Pt1 La1 108.603(6) . 5 ?
La1 Pt1 La1 71.396(6) 81 5 ?
La1 Pt1 La1 108.604(6) 9 5 ?
La1 Pt1 La1 180.0 77 5 ?
O1 Pt1 La1 125.651(4) . 73 ?
O1 Pt1 La1 54.35(6) 81 73 ?
O1 Pt1 La1 125.651(4) 9 73 ?
O1 Pt1 La1 125.88(9) 77 73 ?
O1 Pt1 La1 54.12(9) 5 73 ?
O1 Pt1 La1 54.35(6) 73 73 ?
La1 Pt1 La1 180.0 . 73 ?
La1 Pt1 La1 108.604(6) 81 73 ?
La1 Pt1 La1 71.396(6) 9 73 ?
La1 Pt1 La1 108.604(6) 77 73 ?
La1 Pt1 La1 71.396(6) 5 73 ?
O2 La1 O2 116.180(12) 9 77 ?
O2 La1 O1 76.91(3) 9 77 ?
O2 La1 O1 76.91(3) 77 77 ?
O2 La1 O1 76.91(3) 9 30_455 ?
O2 La1 O1 76.91(3) 77 30_455 ?
O1 La1 O1 129.24(13) 77 30_455 ?
O2 La1 O1 138.04(6) 9 . ?
O2 La1 O1 76.76(7) 77 . ?
O1 La1 O1 67.22(11) 77 . ?
O1 La1 O1 143.56(5) 30_455 . ?
O2 La1 O1 76.76(7) 9 59 ?
O2 La1 O1 138.04(6) 77 59 ?
O1 La1 O1 143.56(5) 77 59 ?
O1 La1 O1 67.22(11) 30_455 59 ?
O1 La1 O1 121.74(14) . 59 ?
O2 La1 O1 138.04(6) 9 52 ?
O2 La1 O1 76.76(7) 77 52 ?
O1 La1 O1 143.56(5) 77 52 ?
O1 La1 O1 67.22(11) 30_455 52 ?
O1 La1 O1 82.52(13) . 52 ?
O1 La1 O1 69.90(13) 59 52 ?
O2 La1 O1 76.76(7) 9 9 ?
O2 La1 O1 138.04(6) 77 9 ?
O1 La1 O1 67.22(11) 77 9 ?
O1 La1 O1 143.56(5) 30_455 9 ?
O1 La1 O1 69.90(13) . 9 ?
O1 La1 O1 82.52(13) 59 9 ?
O1 La1 O1 121.74(14) 52 9 ?
O2 La1 Pt1 97.831(2) 9 28_455 ?
O2 La1 Pt1 97.831(2) 77 28_455 ?
O1 La1 Pt1 169.56(7) 77 28_455 ?
O1 La1 Pt1 40.32(6) 30_455 28_455 ?
O1 La1 Pt1 120.78(7) . 28_455 ?
O1 La1 Pt1 40.30(6) 59 28_455 ?
O1 La1 Pt1 40.30(6) 52 28_455 ?
O1 La1 Pt1 120.78(6) 9 28_455 ?
O2 La1 Pt1 97.831(2) 9 . ?
O2 La1 Pt1 97.831(2) 77 . ?
O1 La1 Pt1 40.32(6) 77 . ?
O1 La1 Pt1 169.56(7) 30_455 . ?
O1 La1 Pt1 40.30(6) . . ?
O1 La1 Pt1 120.78(6) 59 . ?
O1 La1 Pt1 120.78(6) 52 . ?
O1 La1 Pt1 40.30(6) 9 . ?
Pt1 La1 Pt1 150.123(11) 28_455 . ?
O2 La1 K3 58.339(18) 9 73 ?
O2 La1 K3 58.339(18) 77 73 ?
O1 La1 K3 57.8(2) 77 73 ?
O1 La1 K3 71.4(2) 30_455 73 ?
O1 La1 K3 113.92(19) . 73 ?
O1 La1 K3 124.14(17) 59 73 ?
O1 La1 K3 124.14(17) 52 73 ?
O1 La1 K3 113.92(19) 9 73 ?
Pt1 La1 K3 111.7(2) 28_455 73 ?
Pt1 La1 K3 98.2(2) . 73 ?
O2 La1 K3 58.339(18) 9 25_455 ?
O2 La1 K3 58.339(18) 77 25_455 ?
O1 La1 K3 71.4(2) 77 25_455 ?
O1 La1 K3 57.8(2) 30_455 25_455 ?
O1 La1 K3 124.14(17) . 25_455 ?
O1 La1 K3 113.92(19) 59 25_455 ?
O1 La1 K3 113.92(19) 52 25_455 ?
O1 La1 K3 124.14(18) 9 25_455 ?
Pt1 La1 K3 98.2(2) 28_455 25_455 ?
Pt1 La1 K3 111.7(2) . 25_455 ?
K3 La1 K3 13.6(5) 73 25_455 ?
Pt1 O1 K2 176.8(6) . 9 ?
Pt1 O1 La1 85.56(10) . 81 ?
K2 O1 La1 97.6(6) 9 81 ?
Pt1 O1 La1 85.35(6) . . ?
K2 O1 La1 94.53(7) 9 . ?
La1 O1 La1 91.59(7) 81 . ?
Pt1 O1 La1 85.35(6) . 5 ?
K2 O1 La1 94.53(7) 9 5 ?
La1 O1 La1 91.59(7) 81 5 ?
La1 O1 La1 169.91(13) . 5 ?
Pt1 O1 K1 133.40(16) . 9 ?
La1 O1 K1 141.04(14) 81 9 ?
La1 O1 K1 91.77(7) . 9 ?
La1 O1 K1 91.77(7) 5 9 ?
Pt1 O1 K3 162.5(3) . 9 ?
La1 O1 K3 77.0(2) 81 9 ?
La1 O1 K3 95.02(7) . 9 ?
La1 O1 K3 95.02(7) 5 9 ?
K1 O1 K3 64.1(2) 9 9 ?
La1 O2 La1 92.940(3) 34_545 6_556 ?
La1 O2 La1 92.940(3) 34_545 5 ?
La1 O2 La1 153.819(13) 6_556 5 ?
La1 O2 La1 153.819(13) 34_545 81 ?
La1 O2 La1 92.940(3) 6_556 81 ?
La1 O2 La1 92.940(3) 5 81 ?
La1 O2 K3 77.032(11) 34_545 9 ?
La1 O2 K3 110.9(3) 6_556 9 ?
La1 O2 K3 95.3(3) 5 9 ?
La1 O2 K3 77.032(10) 81 9 ?
La1 O2 K3 110.9(3) 34_545 77 ?
La1 O2 K3 77.032(11) 6_556 77 ?
La1 O2 K3 77.032(11) 5 77 ?
La1 O2 K3 95.3(3) 81 77 ?
K3 O2 K3 169.0(4) 9 77 ?
La1 O2 K3 77.032(11) 34_545 57_556 ?
La1 O2 K3 95.3(3) 6_556 57_556 ?
La1 O2 K3 110.9(3) 5 57_556 ?
La1 O2 K3 77.032(10) 81 57_556 ?
K3 O2 K3 169.0(4) 77 57_556 ?
La1 O2 K3 95.3(3) 34_545 29_545 ?
La1 O2 K3 77.032(11) 6_556 29_545 ?
La1 O2 K3 77.032(11) 5 29_545 ?
La1 O2 K3 110.9(3) 81 29_545 ?
K3 O2 K3 169.0(4) 9 29_545 ?
K3 O2 K3 169.0(4) 57_556 29_545 ?
La1 O2 K2 78.35(4) 34_545 9 ?
La1 O2 K2 130.0(4) 6_556 9 ?
La1 O2 K2 76.1(4) 5 9 ?
La1 O2 K2 78.35(4) 81 9 ?
K3 O2 K2 152.0(4) 77 9 ?
K3 O2 K2 152.0(4) 29_545 9 ?
La1 O2 K2 130.0(4) 34_545 77 ?
La1 O2 K2 78.35(4) 6_556 77 ?
La1 O2 K2 78.35(4) 5 77 ?
La1 O2 K2 76.1(4) 81 77 ?
K3 O2 K2 152.0(4) 9 77 ?
K3 O2 K2 152.0(4) 57_556 77 ?
K2 O2 K2 142.6(5) 9 77 ?
La1 O2 K2 78.35(4) 34_545 57_556 ?
La1 O2 K2 76.1(4) 6_556 57_556 ?
La1 O2 K2 130.0(4) 5 57_556 ?
La1 O2 K2 78.35(4) 81 57_556 ?
K3 O2 K2 152.0(4) 77 57_556 ?
K3 O2 K2 152.0(4) 29_545 57_556 ?
K2 O2 K2 53.9(8) 9 57_556 ?
K2 O2 K2 142.6(5) 77 57_556 ?
La1 O2 K2 76.1(4) 34_545 29_545 ?
La1 O2 K2 78.35(4) 6_556 29_545 ?
La1 O2 K2 78.35(4) 5 29_545 ?
La1 O2 K2 130.0(4) 81 29_545 ?
K3 O2 K2 152.0(4) 9 29_545 ?
K3 O2 K2 152.0(4) 57_556 29_545 ?
K2 O2 K2 142.6(5) 9 29_545 ?
K2 O2 K2 53.9(8) 77 29_545 ?
K2 O2 K2 142.6(5) 57_556 29_545 ?
K1 O3 K1 180.0 57 9 ?
K1 O3 K1 90.0 57 49 ?
K1 O3 K1 90.0 9 49 ?
K1 O3 K1 90.0 57 5 ?
K1 O3 K1 90.0 9 5 ?
K1 O3 K1 90.0 49 5 ?
K1 O3 K1 90.0 57 53 ?
K1 O3 K1 90.0 9 53 ?
K1 O3 K1 90.0 49 53 ?
K1 O3 K1 180.0 5 53 ?
K1 O3 K1 90.0 57 . ?
K1 O3 K1 90.0 9 . ?
K1 O3 K1 180.0 49 . ?
K1 O3 K1 90.0 5 . ?
K1 O3 K1 90.0 53 . ?
K2 K1 O3 180.0 . . ?
K2 K1 O1 64.34(9) . 5 ?
O3 K1 O1 115.66(9) . 5 ?
K2 K1 O1 64.34(9) . 6 ?
O3 K1 O1 115.66(9) . 6 ?
O1 K1 O1 128.67(19) 5 6 ?
K2 K1 O1 64.34(9) . 56 ?
O3 K1 O1 115.66(9) . 56 ?
O1 K1 O1 79.19(7) 5 56 ?
O1 K1 O1 79.19(7) 6 56 ?
K2 K1 O1 64.34(9) . 55 ?
O3 K1 O1 115.66(9) . 55 ?
O1 K1 O1 79.19(7) 5 55 ?
O1 K1 O1 79.19(7) 6 55 ?
O1 K1 O1 128.67(19) 56 55 ?
K2 K1 K3 0.0 . . ?
O3 K1 K3 180.0 . . ?
O1 K1 K3 64.34(9) 5 . ?
O1 K1 K3 64.34(9) 6 . ?
O1 K1 K3 64.34(9) 56 . ?
O1 K1 K3 64.34(9) 55 . ?
K2 K1 K1 135.0 . 57 ?
O3 K1 K1 45.0 . 57 ?
O1 K1 K1 139.19(6) 5 57 ?
O1 K1 K1 81.70(8) 6 57 ?
O1 K1 K1 139.19(6) 56 57 ?
O1 K1 K1 81.70(8) 55 57 ?
K3 K1 K1 135.0 . 57 ?
K2 K1 K1 135.0 . 53 ?
O3 K1 K1 45.0 . 53 ?
O1 K1 K1 139.19(6) 5 53 ?
O1 K1 K1 81.70(8) 6 53 ?
O1 K1 K1 81.70(8) 56 53 ?
O1 K1 K1 139.19(6) 55 53 ?
K3 K1 K1 135.0 . 53 ?
K1 K1 K1 60.0 57 53 ?
K2 K1 K1 135.0 . 9 ?
O3 K1 K1 45.0 . 9 ?
O1 K1 K1 81.70(8) 5 9 ?
O1 K1 K1 139.19(6) 6 9 ?
O1 K1 K1 81.70(8) 56 9 ?
O1 K1 K1 139.19(6) 55 9 ?
K3 K1 K1 135.0 . 9 ?
K1 K1 K1 90.0 57 9 ?
K1 K1 K1 60.0 53 9 ?
K2 K1 K1 135.0 . 5 ?
O3 K1 K1 45.0 . 5 ?
O1 K1 K1 81.70(8) 5 5 ?
O1 K1 K1 139.19(6) 6 5 ?
O1 K1 K1 139.19(6) 56 5 ?
O1 K1 K1 81.70(8) 55 5 ?
K3 K1 K1 135.0 . 5 ?
K1 K1 K1 60.0 57 5 ?
K1 K1 K1 90.0 53 5 ?
K1 K1 K1 60.0 9 5 ?
K2 K1 La1 74.63(5) . 9 ?
O3 K1 La1 105.37(5) . 9 ?
O1 K1 La1 43.168(14) 5 9 ?
O1 K1 La1 119.98(9) 6 9 ?
O1 K1 La1 119.98(9) 56 9 ?
O1 K1 La1 43.168(14) 55 9 ?
K3 K1 La1 74.63(5) . 9 ?
K1 K1 La1 100.80(3) 57 9 ?
K1 K1 La1 150.37(5) 53 9 ?
K1 K1 La1 100.80(3) 9 9 ?
K1 K1 La1 60.37(5) 5 9 ?
K3 K2 K1 180.0 . . ?
K3 K2 K3 0.0 . 49_655 ?
K1 K2 K3 180.0 . 49_655 ?
K3 K2 O1 107.7(6) . 6 ?
K1 K2 O1 72.3(6) . 6 ?
K3 K2 O1 107.7(6) 49_655 6 ?
K3 K2 O1 107.7(6) . 5 ?
K1 K2 O1 72.3(6) . 5 ?
K3 K2 O1 107.7(6) 49_655 5 ?
O1 K2 O1 144.5(11) 6 5 ?
K3 K2 O1 107.7(6) . 56 ?
K1 K2 O1 72.3(6) . 56 ?
K3 K2 O1 107.7(6) 49_655 56 ?
O1 K2 O1 84.7(3) 6 56 ?
O1 K2 O1 84.7(3) 5 56 ?
K3 K2 O1 107.7(6) . 55 ?
K1 K2 O1 72.3(6) . 55 ?
K3 K2 O1 107.7(6) 49_655 55 ?
O1 K2 O1 84.7(3) 6 55 ?
O1 K2 O1 84.7(3) 5 55 ?
O1 K2 O1 144.5(11) 56 55 ?
K3 K2 K2 0.0 . 49_655 ?
K1 K2 K2 180.0 . 49_655 ?
K3 K2 K2 0.0 49_655 49_655 ?
O1 K2 K2 107.7(6) 6 49_655 ?
O1 K2 K2 107.7(6) 5 49_655 ?
O1 K2 K2 107.7(6) 56 49_655 ?
O1 K2 K2 107.7(6) 55 49_655 ?
K3 K2 O2 63.1(4) . 81 ?
K1 K2 O2 116.9(4) . 81 ?
K3 K2 O2 63.1(4) 49_655 81 ?
O1 K2 O2 137.6(2) 6 81 ?
O1 K2 O2 62.46(15) 5 81 ?
O1 K2 O2 62.46(15) 56 81 ?
O1 K2 O2 137.6(2) 55 81 ?
K2 K2 O2 63.1(4) 49_655 81 ?
K3 K2 O2 63.1(4) . 5 ?
K1 K2 O2 116.9(4) . 5 ?
K3 K2 O2 63.1(4) 49_655 5 ?
O1 K2 O2 137.6(2) 6 5 ?
O1 K2 O2 62.46(15) 5 5 ?
O1 K2 O2 137.6(2) 56 5 ?
O1 K2 O2 62.46(15) 55 5 ?
K2 K2 O2 63.1(4) 49_655 5 ?
O2 K2 O2 78.2(3) 81 5 ?
K3 K2 O2 63.1(4) . 33_544 ?
K1 K2 O2 116.9(4) . 33_544 ?
K3 K2 O2 63.1(4) 49_655 33_544 ?
O1 K2 O2 62.46(15) 6 33_544 ?
O1 K2 O2 137.6(2) 5 33_544 ?
O1 K2 O2 137.6(2) 56 33_544 ?
O1 K2 O2 62.46(15) 55 33_544 ?
K2 K2 O2 63.1(4) 49_655 33_544 ?
O2 K2 O2 126.1(8) 81 33_544 ?
O2 K2 O2 78.2(3) 5 33_544 ?
K3 K2 O2 63.1(4) . 53_655 ?
K1 K2 O2 116.9(4) . 53_655 ?
K3 K2 O2 63.1(4) 49_655 53_655 ?
O1 K2 O2 62.46(15) 6 53_655 ?
O1 K2 O2 137.6(2) 5 53_655 ?
O1 K2 O2 62.46(15) 56 53_655 ?
O1 K2 O2 137.6(2) 55 53_655 ?
K2 K2 O2 63.1(4) 49_655 53_655 ?
O2 K2 O2 78.2(3) 81 53_655 ?
O2 K2 O2 126.1(8) 5 53_655 ?
O2 K2 O2 78.2(3) 33_544 53_655 ?
K3 K3 K2 180.0 49_655 . ?
K3 K3 K2 0.0 49_655 49_655 ?
K2 K3 K2 180.0 . 49_655 ?
K3 K3 K1 180.0 49_655 . ?
K2 K3 K1 0.0 . . ?
K2 K3 K1 180.0 49_655 . ?
K3 K3 O1 128.4(2) 49_655 6 ?
K2 K3 O1 51.6(2) . 6 ?
K2 K3 O1 128.4(2) 49_655 6 ?
K1 K3 O1 51.6(2) . 6 ?
K3 K3 O1 128.4(2) 49_655 56 ?
K2 K3 O1 51.6(2) . 56 ?
K2 K3 O1 128.4(2) 49_655 56 ?
K1 K3 O1 51.6(2) . 56 ?
O1 K3 O1 67.3(2) 6 56 ?
K3 K3 O1 128.4(2) 49_655 55 ?
K2 K3 O1 51.6(2) . 55 ?
K2 K3 O1 128.4(2) 49_655 55 ?
K1 K3 O1 51.6(2) . 55 ?
O1 K3 O1 67.3(2) 6 55 ?
O1 K3 O1 103.2(4) 56 55 ?
K3 K3 O1 128.4(2) 49_655 5 ?
K2 K3 O1 51.6(2) . 5 ?
K2 K3 O1 128.4(2) 49_655 5 ?
K1 K3 O1 51.6(2) . 5 ?
O1 K3 O1 103.2(4) 6 5 ?
O1 K3 O1 67.3(2) 56 5 ?
O1 K3 O1 67.3(2) 55 5 ?
K3 K3 O2 82.2(3) 49_655 81 ?
K2 K3 O2 97.8(3) . 81 ?
K2 K3 O2 82.2(3) 49_655 81 ?
K1 K3 O2 97.8(3) . 81 ?
O1 K3 O2 129.3(3) 6 81 ?
O1 K3 O2 62.28(8) 56 81 ?
O1 K3 O2 129.3(3) 55 81 ?
O1 K3 O2 62.28(8) 5 81 ?
K3 K3 O2 82.2(3) 49_655 5 ?
K2 K3 O2 97.8(3) . 5 ?
K2 K3 O2 82.2(3) 49_655 5 ?
K1 K3 O2 97.8(3) . 5 ?
O1 K3 O2 129.3(3) 6 5 ?
O1 K3 O2 129.3(3) 56 5 ?
O1 K3 O2 62.28(8) 55 5 ?
O1 K3 O2 62.28(8) 5 5 ?
O2 K3 O2 88.95(7) 81 5 ?
K3 K3 O2 82.2(3) 49_655 33_544 ?
K2 K3 O2 97.8(3) . 33_544 ?
K2 K3 O2 82.2(3) 49_655 33_544 ?
K1 K3 O2 97.8(3) . 33_544 ?
O1 K3 O2 62.28(8) 6 33_544 ?
O1 K3 O2 129.3(3) 56 33_544 ?
O1 K3 O2 62.28(8) 55 33_544 ?
O1 K3 O2 129.3(3) 5 33_544 ?
O2 K3 O2 164.5(5) 81 33_544 ?
O2 K3 O2 88.95(7) 5 33_544 ?
K3 K3 O2 82.2(3) 49_655 53_655 ?
K2 K3 O2 97.8(3) . 53_655 ?
K2 K3 O2 82.2(3) 49_655 53_655 ?
K1 K3 O2 97.8(3) . 53_655 ?
O1 K3 O2 62.28(8) 6 53_655 ?
O1 K3 O2 62.28(8) 56 53_655 ?
O1 K3 O2 129.3(3) 55 53_655 ?
O1 K3 O2 129.3(3) 5 53_655 ?
O2 K3 O2 88.95(7) 81 53_655 ?
O2 K3 O2 164.5(5) 5 53_655 ?
O2 K3 O2 88.95(7) 33_544 53_655 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pt1 O1 2.041(3) . ?
Pt1 O1 2.041(3) 81 ?
Pt1 O1 2.041(3) 9 ?
Pt1 O1 2.041(3) 77 ?
Pt1 O1 2.041(3) 5 ?
Pt1 O1 2.041(3) 73 ?
Pt1 La1 3.1451(1) . ?
Pt1 La1 3.1451(1) 81 ?
Pt1 La1 3.1451(1) 9 ?
Pt1 La1 3.1451(1) 77 ?
Pt1 La1 3.1451(1) 5 ?
Pt1 La1 3.1451(1) 73 ?
La1 O2 2.53129(17) 9 ?
La1 O2 2.53129(17) 77 ?
La1 O1 2.556(3) 77 ?
La1 O1 2.556(3) 30_455 ?
La1 O1 2.564(2) . ?
La1 O1 2.564(2) 59 ?
La1 O1 2.564(2) 52 ?
La1 O1 2.564(2) 9 ?
La1 Pt1 3.1451(1) 28_455 ?
La1 K3 3.5113(17) 73 ?
La1 K3 3.5113(17) 25_455 ?
O1 K2 2.511(8) 9 ?
O1 La1 2.556(3) 81 ?
O1 La1 2.564(2) 5 ?
O1 K1 2.653(3) 9 ?
O1 K3 3.051(9) 9 ?
O2 La1 2.53127(17) 34_545 ?
O2 La1 2.53127(17) 6_556 ?
O2 La1 2.53127(17) 5 ?
O2 La1 2.53127(17) 81 ?
O2 K3 3.0670(19) 9 ?
O2 K3 3.0670(19) 77 ?
O2 K3 3.0670(19) 57_556 ?
O2 K3 3.0670(19) 29_545 ?
O2 K2 3.409(12) 9 ?
O2 K2 3.409(12) 77 ?
O2 K2 3.409(12) 57_556 ?
O2 K2 3.409(12) 29_545 ?
O3 K1 2.619(3) 57 ?
O3 K1 2.619(3) 9 ?
O3 K1 2.619(3) 49 ?
O3 K1 2.619(3) 5 ?
O3 K1 2.619(3) 53 ?
O3 K1 2.619(3) . ?
K1 K2 1.91(3) . ?
K1 O1 2.653(3) 5 ?
K1 O1 2.653(3) 6 ?
K1 O1 2.653(3) 56 ?
K1 O1 2.653(3) 55 ?
K1 K3 3.044(14) . ?
K1 K1 3.704(5) 57 ?
K1 K1 3.704(5) 53 ?
K1 K1 3.704(5) 9 ?
K1 K1 3.704(5) 5 ?
K1 La1 3.7461(9) 9 ?
K2 K3 1.13(2) . ?
K2 K3 1.96(3) 49_655 ?
K2 O1 2.511(8) 6 ?
K2 O1 2.511(8) 5 ?
K2 O1 2.511(8) 56 ?
K2 O1 2.511(8) 55 ?
K2 K2 3.09(5) 49_655 ?
K2 O2 3.409(12) 81 ?
K2 O2 3.409(12) 5 ?
K2 O2 3.409(12) 33_544 ?
K2 O2 3.409(12) 53_655 ?
K3 K3 0.83(3) 49_655 ?
K3 K2 1.96(3) 49_655 ?
K3 O1 3.051(9) 6 ?
K3 O1 3.051(9) 56 ?
K3 O1 3.051(9) 55 ?
K3 O1 3.051(9) 5 ?
K3 O2 3.0670(19) 81 ?
K3 O2 3.0670(19) 5 ?
K3 O2 3.0670(19) 33_544 ?
K3 O2 3.0670(19) 53_655 ?
